Download presentation

Presentation is loading. Please wait.

Published byHunter Cheever Modified about 1 year ago

1
ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties vary with the sample orientation? TOPIC 3: STRUCTURE OF SOLIDS Based on Chapter 3 (Callister)

2
Dense, regular packing Dense, regular-packed structures tend to have lower energy ENERGY AND PACKING Non dense, random packing

3
SOME DEFINITIONS … Lattice: 3D array of regularly spaced points Crystalline material: atoms situated in a repeating 3D periodic array over large atomic distances Amorphous material: material with no such order Hard sphere representation: atoms denoted by hard, touching spheres Reduced sphere representation Unit cell: basic building block unit (such as a flooring tile) that repeats in space to create the crystal structure; it is usually a parallelepiped or prizm

4
tend to be densely packed. have several reasons for dense packing: -Typically, made of heavy element. -Metallic bonding is not directional; i.e., no restrictions as to the number and position of nearest-neighbor atoms -Nearest neighbor distances tend to be small in order to lower bond energy. have the simplest crystal structures. We will look at four such structures... METALLIC CRYSTALS

5
POLYCRYSTALLINE MATERIALS “Nuclei” form during solidification, each of which grows into crystals

6
ATOMIC PACKING FACTOR Fill a box with hard spheres –Packing factor = total volume of spheres in box / volume of box –Question: what is the maximum packing factor you can expect? In crystalline materials: –Atomic packing factor = total volume of atoms in unit cell / volume of unit cell –(as unit cell repeats in space)

7
Atomic packing factor In crystallography, atomic packing factor (APF) or packing fraction is the fraction of volume in acrystal structure that is occupied by atoms. It is dimensionless and always less than unity. For one-component crystals (those that contain only one type of atom), the APF is represented mathematically by where Natoms is the number of atoms in the crystal, Vatom is the volume of an atom, and Vcrystal is the volume occupied by the crystal. It can be proven mathematically that for one-component structures, the most dense arrangement of atoms has an APF of about In reality, this number can be higher due to specific intermolecular factors. For multiple-component structures, the APF can exceed APF = Volume of atoms in unit cell* Volume of unit cell *assume hard spheres

8
APF for a simple cubic structure = 0.52 ATOMIC PACKING FACTOR contains 8 x 1/8 = 1atom/unit cell Adapted from Fig. 3.19, Callister 6e. Lattice constant close-packed directions a R=0.5a

9
Cubic unit cell is 3D repeat unit Rare (only Po has this structure) Close-packed directions (directions along which atoms touch each other) are cube edges. Coordination # = 6 (# nearest neighbors) (Courtesy P.M. Anderson) SIMPLE CUBIC STRUCTURE (SC)

10
Coordination # = 8 Adapted from Fig. 3.2, Callister 6e. (Courtesy P.M. Anderson) Close packed directions are cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. BODY CENTERED CUBIC STRUCTURE (BCC)

11
APF for a body-centered cubic structure = 3/8 = 0.68 Adapted from Fig. 3.2, Callister 6e. ATOMIC PACKING FACTOR: BCC

12
Coordination # = 12 Adapted from Fig. 3.1(a), Callister 6e. (Courtesy P.M. Anderson) Close packed directions are face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. FACE CENTERED CUBIC STRUCTURE (FCC)

13
APF for a body-centered cubic structure = /(3 2) = 0.74 (best possible packing of identical spheres) Adapted from Fig. 3.1(a), Callister 6e. ATOMIC PACKING FACTOR: FCC

14
ABCABC... Stacking Sequence FCC Unit Cell FCC STACKING SEQUENCE 2D Projection

15
HEXAGONAL CLOSE-PACKED STRUCTURE (HCP) Ideally, c/a = for close packing However, in most metals, c/a ratio deviates from this value

16
Coordination # = 12 ABAB... Stacking Sequence APF = 0.74, for ideal c/a ratio of D Projection 2D Projection Adapted from Fig. 3.3, Callister 6e. HEXAGONAL CLOSE-PACKED STRUCTURE (HCP)

17
Close packed crystals A plane B plane C plane A plane …ABCABCABC… packing [Face Centered Cubic (FCC)] …ABABAB… packing [Hexagonal Close Packing (HCP)]

18

19
Slide 11 of 46

20
Slide 12 of 46

21

22
COMPARISON OF CRYSTAL STRUCTURES Crystal structurecoordination #packing factorclose packed directions Simple Cubic (SC)60.52cube edges Body Centered Cubic (BCC)80.68body diagonal Face Centered Cubic (FCC)120.74face diagonal Hexagonal Close Pack (HCP)120.74hexagonal side

23
THEORETICAL DENSITY, Density = mass/volume mass = number of atoms per unit cell * mass of each atom mass of each atom = atomic weight/avogadro’s number

24
Adapted from Table, "Charac- teristics of Selected Elements", inside front cover, Callister 6e. Characteristics of Selected Elements at 20C

25
Example: Copper Data from Table inside front cover of Callister (see previous slide): crystal structure = FCC: 4 atoms/unit cell atomic weight = g/mol (1 amu = 1 g/mol) atomic radius R = nm (1 nm = 10 cm) -7 THEORETICAL DENSITY,

26
Why? Metals have... close-packing (metallic bonding) large atomic mass Ceramics have... less dense packing (covalent bonding) often lighter elements Polymers have... poor packing (often amorphous) lighter elements (C,H,O) Composites have... intermediate values Data from Table B1, Callister 6e. DENSITIES OF MATERIAL CLASSES metals > ceramics > polymers

27
CRYSTAL SYSTEMS Based on shape of unit cell ignoring actual atomic locations Unit cell = 3-dimensional unit that repeats in space Unit cell geometry completely specified by a, b, c & lattice parameters or lattice constants) Seven possible combinations of a, b, c & , resulting in seven crystal systems

28
CRYSTAL SYSTEMS

29
Structure of NaCl STRUCTURE OF OTHER SYSTEMS (Courtesy P.M. Anderson) Structure of Carbon Graphite Diamond

30
CRYSTAL STRUCTURES Plenty of crystal structures available at: Polymorphism –Same compound occurring in more than one crystal structure Allotropy –Polymorphism in elemental solids (e.g., carbon)

31
CRYSTALLOGRAPHIC POINTS, DIRECTIONS & PLANES In crystalline materials, often necessary to specify points, directions and planes within unit cell and in crystal lattice Three numbers (or indices) used to designate points, directions (lines) or planes, based on basic geometric notions The three indices are determined by placing the origin at one of the corners of the unit cell, and the coordinate axes along the unit cell edges

32
POINT COORDINATES Any point within a unit cell specified as fractional multiples of the unit cell edge lengths Position P specified as q r s; convention: coordinates not separated by commas or punctuation marks

33
EXAMPLE: POINT COORDINATES Locate the point (1/4 1 ½) Specify point coordinates for all atom positions for a BCC unit cell –Answer: 0 0 0, 1 0 0, 1 1 0, 0 1 0, ½ ½ ½, 0 0 1, 1 0 1, 1 1 1, 0 1 1

34
CRYSTALLOGRAPHIC DIRECTIONS Defined as line between two points: a vector Steps for finding the 3 indices denoting a direction –Determine the point positions of a beginning point (X1 Y1 Z1) and a ending point (X2 Y2 Z2) for direction, in terms of unit cell edges –Calculate difference between ending and starting point –Multiply the differences by a common constant to convert them to the smallest possible integers u, v, w –The three indices are not separated by commas and are enclosed in square brackets: [uvw] –If any of the indices is negative, a bar is placed in top of that index

35
COMMON DIRECTIONS

36
EXAMPLES: DIRECTIONS Draw a [1,-1,0] direction within a cubic unit cell Determine the indices for this direction –Answer: [120]

37
CRYSTALLOGRAPHIC PLANES Crystallographic planes specified by 3 Miller indices as (hkl) Procedure for determining h,k and l: –If plane passes through origin, translate plane or choose new origin –Determine intercepts of planes on each of the axes in terms of unit cell edge lengths (lattice parameters). Note: if plane has no intercept to an axis (i.e., it is parallel to that axis), intercept is infinity (½ ¼ ½) –Determine reciprocal of the three intercepts (2 4 2) –If necessary, multiply these three numbers by a common factor which converts all the reciprocals to small integers (1 2 1) –The three indices are not separated by commas and are enclosed in curved brackets: (hkl) (121) –If any of the indices is negative, a bar is placed in top of that index

38
THREE IMPORTANT CRYSTAL PLANES

39
Parallel planes are equivalent

40
EXAMPLE: CRYSTAL PLANES Construct a (0,-1,1) plane

41
FCC & BCC CRYSTAL PLANES Consider (110) plane Atomic packing different in the two cases Family of planes: all planes that are crystallographically equivalent—that is having the same atomic packing, indicated as {hkl} –For example, {100} includes (100), (010), (001) planes –{110} includes (110), (101), (011), etc.

42
LINEAR & PLANAR DENSITIES Linear density (LD) = number of atoms centered on a direction vector / length of direction vector –LD (110) = 2 atoms/(4R) = 1/(2R) Planar density (PD) = number of atoms centered on a plane / area of plane –PD (110) = 2 atoms / [(4R)(2R 2)] = 2 atoms / (8R 2 2) = 1/(4R 2 2) LD and PD are important considerations during deformation and “slip”; planes tend to slip or slide along planes with high PD along directions with high LD

43
Some engineering applications require single crystals: Crystal properties reveal features of atomic structure. (Courtesy P.M. Anderson) --Ex: Certain crystal planes in quartz fracture more easily than others. --diamond single crystals for abrasives --turbine blades Fig. 8.30(c), Callister 6e. (Fig. 8.30(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) CRYSTALS AS BUILDING BLOCKS Single crystal: when the periodic and repeated arrangement of atoms is perfect and extends throughout the entirety of the specimen

44
POLYCRYSTALLINE MATERIALS “Nuclei” form during solidification, each of which grows into crystals

45
Most engineering materials are polycrystals. Nb-Hf-W plate with an electron beam weld. Each "grain" is a single crystal. If crystals are randomly oriented, overall component properties are not directional. Crystal sizes typ. range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers). Adapted from Fig. K, color inset pages of Callister 6e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm POLYCRYSTALS

46
Single Crystals -Properties vary with direction: anisotropic. -Example: the modulus of elasticity (E) in BCC iron: Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (E poly iron = 210 GPa) -If grains are textured, anisotropic. 200 mm Data from Table 3.3, Callister 6e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) Adapted from Fig. 4.12(b), Callister 6e. (Fig. 4.12(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].) SINGLE VS POLYCRYSTALS

47
atoms pack in periodic, 3D arrays typical of: Crystalline materials... -metals -many ceramics -some polymers atoms have no periodic packing occurs for: Noncrystalline materials... -complex structures -rapid cooling crystalline SiO 2 noncrystalline SiO 2 "Amorphous" = Noncrystalline Adapted from Fig. 3.18(b), Callister 6e. Adapted from Fig. 3.18(a), Callister 6e. AMORPHOUS MATERIALS

48
Incoming X-rays diffract from crystal planes, following Braggs law: n = 2dsin( ) Measurement of: Critical angles, c, for X-rays provide atomic spacing, d. Adapted from Fig. 3.2W, Callister 6e. X-RAYS TO CONFIRM CRYSTAL STRUCTURE

49
Atoms can be arranged and imaged! Carbon monoxide molecules arranged on a platinum (111) surface. Photos produced from the work of C.P. Lutz, Zeppenfeld, and D.M. Eigler. Reprinted with permission from International Business Machines Corporation, copyright Iron atoms arranged on a copper (111) surface. These Kanji characters represent the word “atom”. SCANNING TUNNELING MICROSCOPY

50
Atoms may assemble into crystalline, polycrystalline or amorphous structures. We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but properties are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. SUMMARY

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google